Electronic supplementary Electronic supplementary information Mesoporous Iron Oxide Nanowires:...
Embed Size (px)
Transcript of Electronic supplementary Electronic supplementary information Mesoporous Iron Oxide Nanowires:...
Electronic supplementary information
Mesoporous Iron Oxide Nanowires: Synthesis, Magnetic and Photocatalytic Properties
Kinjal Gandha,a Jeotikanta Mohapatra,a Mohammad Kabir Hossain,b Kevin Elkins,a Narayan Poudyal,a Krishnan Rajeshwar,b and J. Ping Liua*
aDepartment of Physics, University of Texas at Arlington, Arlington, Texas 76019, USA bDepartment of Chemistry and Biochemistry, University of Texas at Arlington, Arlington, Texas 76019, USA
*To whom correspondence should be addressed. E-mail: email@example.com (J. Ping Liu). Phone: +1-817- 272-2815
Fig. S1: XRD pattern of NWs samples produced by annealing FeOOH NWs at 400 °C. A
mixture of Fe3O4 and Fe phases is confirmed.
Electronic Supplementary Material (ESI) for RSC Advances. This journal is © The Royal Society of Chemistry 2016
Fig. S2: HRSEM images of as-prepared (a) FeOOH NWs, (b) α-Fe2O3 NWs, (c) Fe3O4 NWs,
and (d) α-Fe NWs.
2 3 4 5
Fe2O3/ZnO Fe2O3 ZnO
Fig. S3: Calculation of the band gap from the UV-visible absorption spectra. The band gap
energies estimated from the intercept of the tangents to the plots were 3.1, 2.2 and 2.5 eV for the
ZnO nanoparticles, α-Fe2O3 NWs and α-Fe2O3/ZnO NNHs respectively.
Fig. S4: Photographs showing complete decolorization of (a) Rhodamine B, (b) methyl orange
and (c) methylene blue under visible light for 90 min. The initial concentration/loading of the
dye and photocatalyst (α-Fe2O3/ZnO NNHs) were 20 µM and 40 mg, respectively.
0 20 40 60 80 0.0
ZnO Nanoparticles Comercial Fe2O3 Fe2O3 NWs ZnO/Fe2O3 NNHs
C/ C 0
Fig S5: Comparison of photocatalytic activity of α-Fe2O3/ZnO NNHs with pristine ZnO
nanoparticles, commercial α-Fe2O3, α-Fe2O3 NWs. The photocatalytic activity measurement was
performed under identical conditions (equivalent catalyst concentration, temperature and oxygen
Fig. S6: Absorption spectra for (a) MB and (b) MO dyes as a function of irradiation time of
simulated solar light in the presence of ɑ-Fe2O3/ZnO NNHs (40 mg). The initial concentration of
dye used for the photodegradation experiment was 20 µM. (c) Degradation efficiency of ɑ-
Fe2O3/ZnO NNHs with different ZnO nanoparticles loading and commercial P-25 TiO2.
Fig S7: Separation of magnetic α-Fe2O3/ZnO NNHs from the solution after photocatalytic
degradation of RhB dye. (a) Initial dye solution 20 µM/ml, (b) α-Fe2O3/ZnO NNHs dispersed in
RhB dye solution and (c) after photocatalytic dye degradation, the α-Fe2O3/ZnO NNHs were
separated from the cleaned water by applying a magnetic field.
Fig S8: SEM images of α-Fe2O3/ZnO NNHs (a) before, and (b) after photocatalytic dye